#------------------------------------------------------------------------------
#$Date: 2023-11-29 05:05:15 +0200 (Wed, 29 Nov 2023) $
#$Revision: 287856 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/30/07/2300726.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2300726
loop_
_publ_author_name
'Ait Haddouch, Mohammed'
'Abboushi, Nour'
'Sharma, Neetika'
'Eich, Andreas'
'Grzechnik, Andrzej'
'Li, Cheng'
'Tolkiehn, Martin'
'Alsamamra, Husain'
'Voigt, Jörg'
'Friese, Karen'
_publ_section_title
;
 Site dependence of the magnetocaloric effect in Mn₅₋ₓ
 Fe ₓ Si₃.
;
_journal_coeditor_code           IU5027SUP1
_journal_issue                   'Pt 5'
_journal_name_full               'Journal of applied crystallography'
_journal_page_first              1164
_journal_page_last               1172
_journal_paper_doi               10.1107/S1600576722007440
_journal_volume                  55
_journal_year                    2022
_chemical_formula_moiety         'Fe2 Mn3 Si3'
_chemical_formula_sum            'Fe2 Mn3 Si3'
_chemical_formula_weight         360.8
_space_group_IT_number           193
_space_group_name_Hall           '-P 6c 2'
_space_group_name_H-M_alt        'P 63/m c m'
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      193
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   6.85340(10)
_cell_length_b                   6.85340(10)
_cell_length_c                   4.75560(10)
_cell_measurement_reflns_used    2010
_cell_measurement_temperature    300
_cell_measurement_theta_max      37.07
_cell_measurement_theta_min      2.12
_cell_volume                     193.441(6)
_computing_cell_refinement       'CrysAlisPro 1.171.40.29a (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.40.29a (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.40.29a (Rigaku OD, 2018)'
_diffrn_ambient_temperature      300
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.99
_diffrn_measured_fraction_theta_max 0.99
_diffrn_measurement_device_type
'esperanto-CrysAlisPro-abstract goniometer imported esperanto images'
_diffrn_measurement_method       'φ scans'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.44279
_diffrn_reflns_av_R_equivalents  0.0556
_diffrn_reflns_av_unetI/netI     0.0183
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            10552
_diffrn_reflns_theta_full        37.41
_diffrn_reflns_theta_max         37.41
_diffrn_reflns_theta_min         2.14
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    4.375
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.059
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.29a (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'metallic black'
_exptl_crystal_density_diffrn    6.1938
_exptl_crystal_description       irregular
_exptl_crystal_F_000             338
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.11
_refine_diff_density_min         -1.53
_refine_ls_extinction_coef       690(80)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.31
_refine_ls_goodness_of_fit_ref   1.27
_refine_ls_number_constraints    2
_refine_ls_number_parameters     12
_refine_ls_number_reflns         787
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0315
_refine_ls_R_factor_gt           0.0245
_refine_ls_shift/su_max          0.0094
_refine_ls_shift/su_mean         0.0037
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0259
_refine_ls_wR_factor_ref         0.0274
_reflns_number_gt                655
_reflns_number_total             787
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            iu5027sup1.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 
;
_cod_original_sg_symbol_Hall     '-P 6c;-2'
_cod_database_code               2300726
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 -x,-y,z+1/2
5 y,-x+y,z+1/2
6 x-y,x,z+1/2
7 y,x,-z+1/2
8 x-y,-y,-z+1/2
9 -x,-x+y,-z+1/2
10 -y,-x,-z
11 -x+y,y,-z
12 x,x-y,-z
13 -x,-y,-z
14 y,-x+y,-z
15 x-y,x,-z
16 x,y,-z+1/2
17 -y,x-y,-z+1/2
18 -x+y,-x,-z+1/2
19 -y,-x,z+1/2
20 -x+y,y,z+1/2
21 x,x-y,z+1/2
22 y,x,z
23 x-y,-y,z
24 -x,-x+y,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.666667 0.333333 0 Uani 0.00619(4) 4 0.7656 d . . .
Mn1 Mn 0.666667 0.333333 0 Uani 0.00619(4) 4 0.2344 d . . .
Mn2 Mn 0.23281(3) 0 0.25 Uani 0.00788(4) 6 0.8437 d . . .
Fe2 Fe 0.23281(3) 0 0.25 Uani 0.00788(4) 6 0.1563 d . . .
Si1 Si 0.59802(6) 0 0.25 Uani 0.00692(8) 6 1 d . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe 0.2193 0.3525 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.2006 0.3019 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Si 0.0321 0.0267 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Fe1 Fe1 Fe1 16_554 . 16_555 180 ?
Fe1 Fe1 Mn1 16_554 . . 0 ?
Fe1 Fe1 Mn1 16_554 . 16_554 0 ?
Fe1 Fe1 Mn1 16_554 . 16_555 180 ?
Fe1 Fe1 Si1 16_554 . . 119.6413(16) ?
Fe1 Fe1 Si1 16_554 . 2_655 119.6413(16) ?
Fe1 Fe1 Si1 16_554 . 3_665 119.641(5) ?
Fe1 Fe1 Si1 16_554 . 4_654 60.3587(16) ?
Fe1 Fe1 Si1 16_554 . 5_664 60.3587(16) ?
Fe1 Fe1 Si1 16_554 . 6_554 60.359(5) ?
Fe1 Fe1 Mn1 16_555 . . 0 ?
Fe1 Fe1 Mn1 16_555 . 16_554 180 ?
Fe1 Fe1 Mn1 16_555 . 16_555 0 ?
Fe1 Fe1 Si1 16_555 . . 60.3587(16) ?
Fe1 Fe1 Si1 16_555 . 2_655 60.3587(16) ?
Fe1 Fe1 Si1 16_555 . 3_665 60.359(5) ?
Fe1 Fe1 Si1 16_555 . 4_654 119.6413(16) ?
Fe1 Fe1 Si1 16_555 . 5_664 119.6413(16) ?
Fe1 Fe1 Si1 16_555 . 6_554 119.641(5) ?
Mn1 Fe1 Mn1 . . 16_554 0 ?
Mn1 Fe1 Mn1 . . 16_555 0 ?
Mn1 Fe1 Si1 . . . 0 ?
Mn1 Fe1 Si1 . . 2_655 0 ?
Mn1 Fe1 Si1 . . 3_665 0 ?
Mn1 Fe1 Si1 . . 4_654 0 ?
Mn1 Fe1 Si1 . . 5_664 0 ?
Mn1 Fe1 Si1 . . 6_554 0 ?
Mn1 Fe1 Mn1 16_554 . 16_555 180 ?
Mn1 Fe1 Si1 16_554 . . 119.6413(16) ?
Mn1 Fe1 Si1 16_554 . 2_655 119.6413(16) ?
Mn1 Fe1 Si1 16_554 . 3_665 119.641(5) ?
Mn1 Fe1 Si1 16_554 . 4_654 60.3587(16) ?
Mn1 Fe1 Si1 16_554 . 5_664 60.3587(16) ?
Mn1 Fe1 Si1 16_554 . 6_554 60.359(5) ?
Mn1 Fe1 Si1 16_555 . . 60.3587(16) ?
Mn1 Fe1 Si1 16_555 . 2_655 60.3587(16) ?
Mn1 Fe1 Si1 16_555 . 3_665 60.359(5) ?
Mn1 Fe1 Si1 16_555 . 4_654 119.6413(16) ?
Mn1 Fe1 Si1 16_555 . 5_664 119.6413(16) ?
Mn1 Fe1 Si1 16_555 . 6_554 119.641(5) ?
Si1 Fe1 Si1 . . 2_655 97.649(9) ?
Si1 Fe1 Si1 . . 3_665 97.649(11) ?
Si1 Fe1 Si1 . . 4_654 69.229(5) ?
Si1 Fe1 Si1 . . 5_664 98.389(12) ?
Si1 Fe1 Si1 . . 6_554 160.482(11) ?
Si1 Fe1 Si1 2_655 . 3_665 97.649(8) ?
Si1 Fe1 Si1 2_655 . 4_654 160.483(12) ?
Si1 Fe1 Si1 2_655 . 5_664 69.229(5) ?
Si1 Fe1 Si1 2_655 . 6_554 98.389(10) ?
Si1 Fe1 Si1 3_665 . 4_654 98.389(10) ?
Si1 Fe1 Si1 3_665 . 5_664 160.482(11) ?
Si1 Fe1 Si1 3_665 . 6_554 69.229(10) ?
Si1 Fe1 Si1 4_654 . 5_664 97.649(9) ?
Si1 Fe1 Si1 4_654 . 6_554 97.649(8) ?
Si1 Fe1 Si1 5_664 . 6_554 97.649(11) ?
Fe1 Mn1 Fe1 . . 16_554 0 ?
Fe1 Mn1 Fe1 . . 16_555 0 ?
Fe1 Mn1 Mn1 . . 16_554 0 ?
Fe1 Mn1 Mn1 . . 16_555 0 ?
Fe1 Mn1 Si1 . . . 0 ?
Fe1 Mn1 Si1 . . 2_655 0 ?
Fe1 Mn1 Si1 . . 3_665 0 ?
Fe1 Mn1 Si1 . . 4_654 0 ?
Fe1 Mn1 Si1 . . 5_664 0 ?
Fe1 Mn1 Si1 . . 6_554 0 ?
Fe1 Mn1 Fe1 16_554 . 16_555 180 ?
Fe1 Mn1 Mn1 16_554 . 16_554 0 ?
Fe1 Mn1 Mn1 16_554 . 16_555 180 ?
Fe1 Mn1 Si1 16_554 . . 119.6413(16) ?
Fe1 Mn1 Si1 16_554 . 2_655 119.6413(16) ?
Fe1 Mn1 Si1 16_554 . 3_665 119.641(5) ?
Fe1 Mn1 Si1 16_554 . 4_654 60.3587(16) ?
Fe1 Mn1 Si1 16_554 . 5_664 60.3587(16) ?
Fe1 Mn1 Si1 16_554 . 6_554 60.359(5) ?
Fe1 Mn1 Mn1 16_555 . 16_554 180 ?
Fe1 Mn1 Mn1 16_555 . 16_555 0 ?
Fe1 Mn1 Si1 16_555 . . 60.3587(16) ?
Fe1 Mn1 Si1 16_555 . 2_655 60.3587(16) ?
Fe1 Mn1 Si1 16_555 . 3_665 60.359(5) ?
Fe1 Mn1 Si1 16_555 . 4_654 119.6413(16) ?
Fe1 Mn1 Si1 16_555 . 5_664 119.6413(16) ?
Fe1 Mn1 Si1 16_555 . 6_554 119.641(5) ?
Mn1 Mn1 Mn1 16_554 . 16_555 180 ?
Mn1 Mn1 Si1 16_554 . . 119.6413(16) ?
Mn1 Mn1 Si1 16_554 . 2_655 119.6413(16) ?
Mn1 Mn1 Si1 16_554 . 3_665 119.641(5) ?
Mn1 Mn1 Si1 16_554 . 4_654 60.3587(16) ?
Mn1 Mn1 Si1 16_554 . 5_664 60.3587(16) ?
Mn1 Mn1 Si1 16_554 . 6_554 60.359(5) ?
Mn1 Mn1 Si1 16_555 . . 60.3587(16) ?
Mn1 Mn1 Si1 16_555 . 2_655 60.3587(16) ?
Mn1 Mn1 Si1 16_555 . 3_665 60.359(5) ?
Mn1 Mn1 Si1 16_555 . 4_654 119.6413(16) ?
Mn1 Mn1 Si1 16_555 . 5_664 119.6413(16) ?
Mn1 Mn1 Si1 16_555 . 6_554 119.641(5) ?
Si1 Mn1 Si1 . . 2_655 97.649(9) ?
Si1 Mn1 Si1 . . 3_665 97.649(11) ?
Si1 Mn1 Si1 . . 4_654 69.229(5) ?
Si1 Mn1 Si1 . . 5_664 98.389(12) ?
Si1 Mn1 Si1 . . 6_554 160.482(11) ?
Si1 Mn1 Si1 2_655 . 3_665 97.649(8) ?
Si1 Mn1 Si1 2_655 . 4_654 160.483(12) ?
Si1 Mn1 Si1 2_655 . 5_664 69.229(5) ?
Si1 Mn1 Si1 2_655 . 6_554 98.389(10) ?
Si1 Mn1 Si1 3_665 . 4_654 98.389(10) ?
Si1 Mn1 Si1 3_665 . 5_664 160.482(11) ?
Si1 Mn1 Si1 3_665 . 6_554 69.229(10) ?
Si1 Mn1 Si1 4_654 . 5_664 97.649(9) ?
Si1 Mn1 Si1 4_654 . 6_554 97.649(8) ?
Si1 Mn1 Si1 5_664 . 6_554 97.649(11) ?
Mn2 Mn2 Mn2 2_555 . 3_555 60.000(7) ?
Mn2 Mn2 Mn2 2_555 . 5_554 90.000(7) ?
Mn2 Mn2 Mn2 2_555 . 5_555 90.000(7) ?
Mn2 Mn2 Mn2 2_555 . 6_554 61.148(6) ?
Mn2 Mn2 Mn2 2_555 . 6_555 61.148(6) ?
Mn2 Mn2 Fe2 2_555 . . 0 ?
Mn2 Mn2 Fe2 2_555 . 2_555 0 ?
Mn2 Mn2 Fe2 2_555 . 3_555 60.000(7) ?
Mn2 Mn2 Fe2 2_555 . 5_554 90.000(7) ?
Mn2 Mn2 Fe2 2_555 . 5_555 90.000(7) ?
Mn2 Mn2 Fe2 2_555 . 6_554 61.148(6) ?
Mn2 Mn2 Fe2 2_555 . 6_555 61.148(6) ?
Mn2 Mn2 Si1 2_555 . . 150.000(3) ?
Mn2 Mn2 Si1 2_555 . 2_545 114.777(10) ?
Mn2 Mn2 Si1 2_555 . 3_665 54.777(11) ?
Mn2 Mn2 Si1 2_555 . 4_654 112.306(7) ?
Mn2 Mn2 Si1 2_555 . 4_655 112.306(7) ?
Mn2 Mn2 Mn2 3_555 . 5_554 61.148(4) ?
Mn2 Mn2 Mn2 3_555 . 5_555 61.148(4) ?
Mn2 Mn2 Mn2 3_555 . 6_554 90.000(7) ?
Mn2 Mn2 Mn2 3_555 . 6_555 90.000(7) ?
Mn2 Mn2 Fe2 3_555 . . 0 ?
Mn2 Mn2 Fe2 3_555 . 2_555 60.000(7) ?
Mn2 Mn2 Fe2 3_555 . 3_555 0 ?
Mn2 Mn2 Fe2 3_555 . 5_554 61.148(4) ?
Mn2 Mn2 Fe2 3_555 . 5_555 61.148(4) ?
Mn2 Mn2 Fe2 3_555 . 6_554 90.000(7) ?
Mn2 Mn2 Fe2 3_555 . 6_555 90.000(7) ?
Mn2 Mn2 Si1 3_555 . . 150.000(6) ?
Mn2 Mn2 Si1 3_555 . 2_545 54.777(8) ?
Mn2 Mn2 Si1 3_555 . 3_665 114.777(13) ?
Mn2 Mn2 Si1 3_555 . 4_654 112.306(7) ?
Mn2 Mn2 Si1 3_555 . 4_655 112.306(7) ?
Mn2 Mn2 Mn2 5_554 . 5_555 112.275(5) ?
Mn2 Mn2 Mn2 5_554 . 6_554 57.704(5) ?
Mn2 Mn2 Mn2 5_554 . 6_555 147.647(10) ?
Mn2 Mn2 Fe2 5_554 . . 0 ?
Mn2 Mn2 Fe2 5_554 . 2_555 90.000(7) ?
Mn2 Mn2 Fe2 5_554 . 3_555 61.148(4) ?
Mn2 Mn2 Fe2 5_554 . 5_554 0 ?
Mn2 Mn2 Fe2 5_554 . 5_555 112.275(5) ?
Mn2 Mn2 Fe2 5_554 . 6_554 57.704(5) ?
Mn2 Mn2 Fe2 5_554 . 6_555 147.647(10) ?
Mn2 Mn2 Si1 5_554 . . 106.177(5) ?
Mn2 Mn2 Si1 5_554 . 2_545 59.608(4) ?
Mn2 Mn2 Si1 5_554 . 3_665 117.077(6) ?
Mn2 Mn2 Si1 5_554 . 4_654 51.371(6) ?
Mn2 Mn2 Si1 5_554 . 4_655 150.283(5) ?
Mn2 Mn2 Mn2 5_555 . 6_554 147.647(10) ?
Mn2 Mn2 Mn2 5_555 . 6_555 57.704(5) ?
Mn2 Mn2 Fe2 5_555 . . 0 ?
Mn2 Mn2 Fe2 5_555 . 2_555 90.000(7) ?
Mn2 Mn2 Fe2 5_555 . 3_555 61.148(4) ?
Mn2 Mn2 Fe2 5_555 . 5_554 112.275(5) ?
Mn2 Mn2 Fe2 5_555 . 5_555 0 ?
Mn2 Mn2 Fe2 5_555 . 6_554 147.647(10) ?
Mn2 Mn2 Fe2 5_555 . 6_555 57.704(5) ?
Mn2 Mn2 Si1 5_555 . . 106.177(5) ?
Mn2 Mn2 Si1 5_555 . 2_545 59.608(4) ?
Mn2 Mn2 Si1 5_555 . 3_665 117.077(6) ?
Mn2 Mn2 Si1 5_555 . 4_654 150.283(5) ?
Mn2 Mn2 Si1 5_555 . 4_655 51.371(6) ?
Mn2 Mn2 Mn2 6_554 . 6_555 112.275(7) ?
Mn2 Mn2 Fe2 6_554 . . 0 ?
Mn2 Mn2 Fe2 6_554 . 2_555 61.148(6) ?
Mn2 Mn2 Fe2 6_554 . 3_555 90.000(7) ?
Mn2 Mn2 Fe2 6_554 . 5_554 57.704(5) ?
Mn2 Mn2 Fe2 6_554 . 5_555 147.647(10) ?
Mn2 Mn2 Fe2 6_554 . 6_554 0 ?
Mn2 Mn2 Fe2 6_554 . 6_555 112.275(7) ?
Mn2 Mn2 Si1 6_554 . . 106.177(6) ?
Mn2 Mn2 Si1 6_554 . 2_545 117.077(5) ?
Mn2 Mn2 Si1 6_554 . 3_665 59.608(4) ?
Mn2 Mn2 Si1 6_554 . 4_654 51.371(8) ?
Mn2 Mn2 Si1 6_554 . 4_655 150.283(4) ?
Mn2 Mn2 Fe2 6_555 . . 0 ?
Mn2 Mn2 Fe2 6_555 . 2_555 61.148(6) ?
Mn2 Mn2 Fe2 6_555 . 3_555 90.000(7) ?
Mn2 Mn2 Fe2 6_555 . 5_554 147.647(10) ?
Mn2 Mn2 Fe2 6_555 . 5_555 57.704(5) ?
Mn2 Mn2 Fe2 6_555 . 6_554 112.275(7) ?
Mn2 Mn2 Fe2 6_555 . 6_555 0 ?
Mn2 Mn2 Si1 6_555 . . 106.177(6) ?
Mn2 Mn2 Si1 6_555 . 2_545 117.077(5) ?
Mn2 Mn2 Si1 6_555 . 3_665 59.608(4) ?
Mn2 Mn2 Si1 6_555 . 4_654 150.283(4) ?
Mn2 Mn2 Si1 6_555 . 4_655 51.371(8) ?
Fe2 Mn2 Fe2 . . 2_555 0 ?
Fe2 Mn2 Fe2 . . 3_555 0 ?
Fe2 Mn2 Fe2 . . 5_554 0 ?
Fe2 Mn2 Fe2 . . 5_555 0 ?
Fe2 Mn2 Fe2 . . 6_554 0 ?
Fe2 Mn2 Fe2 . . 6_555 0 ?
Fe2 Mn2 Si1 . . . 0 ?
Fe2 Mn2 Si1 . . 2_545 0 ?
Fe2 Mn2 Si1 . . 3_665 0 ?
Fe2 Mn2 Si1 . . 4_654 0 ?
Fe2 Mn2 Si1 . . 4_655 0 ?
Fe2 Mn2 Fe2 2_555 . 3_555 60.000(7) ?
Fe2 Mn2 Fe2 2_555 . 5_554 90.000(7) ?
Fe2 Mn2 Fe2 2_555 . 5_555 90.000(7) ?
Fe2 Mn2 Fe2 2_555 . 6_554 61.148(6) ?
Fe2 Mn2 Fe2 2_555 . 6_555 61.148(6) ?
Fe2 Mn2 Si1 2_555 . . 150.000(3) ?
Fe2 Mn2 Si1 2_555 . 2_545 114.777(10) ?
Fe2 Mn2 Si1 2_555 . 3_665 54.777(11) ?
Fe2 Mn2 Si1 2_555 . 4_654 112.306(7) ?
Fe2 Mn2 Si1 2_555 . 4_655 112.306(7) ?
Fe2 Mn2 Fe2 3_555 . 5_554 61.148(4) ?
Fe2 Mn2 Fe2 3_555 . 5_555 61.148(4) ?
Fe2 Mn2 Fe2 3_555 . 6_554 90.000(7) ?
Fe2 Mn2 Fe2 3_555 . 6_555 90.000(7) ?
Fe2 Mn2 Si1 3_555 . . 150.000(6) ?
Fe2 Mn2 Si1 3_555 . 2_545 54.777(8) ?
Fe2 Mn2 Si1 3_555 . 3_665 114.777(13) ?
Fe2 Mn2 Si1 3_555 . 4_654 112.306(7) ?
Fe2 Mn2 Si1 3_555 . 4_655 112.306(7) ?
Fe2 Mn2 Fe2 5_554 . 5_555 112.275(5) ?
Fe2 Mn2 Fe2 5_554 . 6_554 57.704(5) ?
Fe2 Mn2 Fe2 5_554 . 6_555 147.647(10) ?
Fe2 Mn2 Si1 5_554 . . 106.177(5) ?
Fe2 Mn2 Si1 5_554 . 2_545 59.608(4) ?
Fe2 Mn2 Si1 5_554 . 3_665 117.077(6) ?
Fe2 Mn2 Si1 5_554 . 4_654 51.371(6) ?
Fe2 Mn2 Si1 5_554 . 4_655 150.283(5) ?
Fe2 Mn2 Fe2 5_555 . 6_554 147.647(10) ?
Fe2 Mn2 Fe2 5_555 . 6_555 57.704(5) ?
Fe2 Mn2 Si1 5_555 . . 106.177(5) ?
Fe2 Mn2 Si1 5_555 . 2_545 59.608(4) ?
Fe2 Mn2 Si1 5_555 . 3_665 117.077(6) ?
Fe2 Mn2 Si1 5_555 . 4_654 150.283(5) ?
Fe2 Mn2 Si1 5_555 . 4_655 51.371(6) ?
Fe2 Mn2 Fe2 6_554 . 6_555 112.275(7) ?
Fe2 Mn2 Si1 6_554 . . 106.177(6) ?
Fe2 Mn2 Si1 6_554 . 2_545 117.077(5) ?
Fe2 Mn2 Si1 6_554 . 3_665 59.608(4) ?
Fe2 Mn2 Si1 6_554 . 4_654 51.371(8) ?
Fe2 Mn2 Si1 6_554 . 4_655 150.283(4) ?
Fe2 Mn2 Si1 6_555 . . 106.177(6) ?
Fe2 Mn2 Si1 6_555 . 2_545 117.077(5) ?
Fe2 Mn2 Si1 6_555 . 3_665 59.608(4) ?
Fe2 Mn2 Si1 6_555 . 4_654 150.283(4) ?
Fe2 Mn2 Si1 6_555 . 4_655 51.371(8) ?
Si1 Mn2 Si1 . . 2_545 95.223(8) ?
Si1 Mn2 Si1 . . 3_665 95.223(11) ?
Si1 Mn2 Si1 . . 4_654 64.006(9) ?
Si1 Mn2 Si1 . . 4_655 64.006(9) ?
Si1 Mn2 Si1 2_545 . 3_665 169.555(15) ?
Si1 Mn2 Si1 2_545 . 4_654 92.286(3) ?
Si1 Mn2 Si1 2_545 . 4_655 92.286(3) ?
Si1 Mn2 Si1 3_665 . 4_654 92.286(5) ?
Si1 Mn2 Si1 3_665 . 4_655 92.286(5) ?
Si1 Mn2 Si1 4_654 . 4_655 128.013(14) ?
Mn2 Fe2 Mn2 . . 2_555 0 ?
Mn2 Fe2 Mn2 . . 3_555 0 ?
Mn2 Fe2 Mn2 . . 5_554 0 ?
Mn2 Fe2 Mn2 . . 5_555 0 ?
Mn2 Fe2 Mn2 . . 6_554 0 ?
Mn2 Fe2 Mn2 . . 6_555 0 ?
Mn2 Fe2 Fe2 . . 2_555 0 ?
Mn2 Fe2 Fe2 . . 3_555 0 ?
Mn2 Fe2 Fe2 . . 5_554 0 ?
Mn2 Fe2 Fe2 . . 5_555 0 ?
Mn2 Fe2 Fe2 . . 6_554 0 ?
Mn2 Fe2 Fe2 . . 6_555 0 ?
Mn2 Fe2 Si1 . . . 0 ?
Mn2 Fe2 Si1 . . 2_545 0 ?
Mn2 Fe2 Si1 . . 3_665 0 ?
Mn2 Fe2 Si1 . . 4_654 0 ?
Mn2 Fe2 Si1 . . 4_655 0 ?
Mn2 Fe2 Mn2 2_555 . 3_555 60.000(7) ?
Mn2 Fe2 Mn2 2_555 . 5_554 90.000(7) ?
Mn2 Fe2 Mn2 2_555 . 5_555 90.000(7) ?
Mn2 Fe2 Mn2 2_555 . 6_554 61.148(6) ?
Mn2 Fe2 Mn2 2_555 . 6_555 61.148(6) ?
Mn2 Fe2 Fe2 2_555 . 2_555 0 ?
Mn2 Fe2 Fe2 2_555 . 3_555 60.000(7) ?
Mn2 Fe2 Fe2 2_555 . 5_554 90.000(7) ?
Mn2 Fe2 Fe2 2_555 . 5_555 90.000(7) ?
Mn2 Fe2 Fe2 2_555 . 6_554 61.148(6) ?
Mn2 Fe2 Fe2 2_555 . 6_555 61.148(6) ?
Mn2 Fe2 Si1 2_555 . . 150.000(3) ?
Mn2 Fe2 Si1 2_555 . 2_545 114.777(10) ?
Mn2 Fe2 Si1 2_555 . 3_665 54.777(11) ?
Mn2 Fe2 Si1 2_555 . 4_654 112.306(7) ?
Mn2 Fe2 Si1 2_555 . 4_655 112.306(7) ?
Mn2 Fe2 Mn2 3_555 . 5_554 61.148(4) ?
Mn2 Fe2 Mn2 3_555 . 5_555 61.148(4) ?
Mn2 Fe2 Mn2 3_555 . 6_554 90.000(7) ?
Mn2 Fe2 Mn2 3_555 . 6_555 90.000(7) ?
Mn2 Fe2 Fe2 3_555 . 2_555 60.000(7) ?
Mn2 Fe2 Fe2 3_555 . 3_555 0 ?
Mn2 Fe2 Fe2 3_555 . 5_554 61.148(4) ?
Mn2 Fe2 Fe2 3_555 . 5_555 61.148(4) ?
Mn2 Fe2 Fe2 3_555 . 6_554 90.000(7) ?
Mn2 Fe2 Fe2 3_555 . 6_555 90.000(7) ?
Mn2 Fe2 Si1 3_555 . . 150.000(6) ?
Mn2 Fe2 Si1 3_555 . 2_545 54.777(8) ?
Mn2 Fe2 Si1 3_555 . 3_665 114.777(13) ?
Mn2 Fe2 Si1 3_555 . 4_654 112.306(7) ?
Mn2 Fe2 Si1 3_555 . 4_655 112.306(7) ?
Mn2 Fe2 Mn2 5_554 . 5_555 112.275(5) ?
Mn2 Fe2 Mn2 5_554 . 6_554 57.704(5) ?
Mn2 Fe2 Mn2 5_554 . 6_555 147.647(10) ?
Mn2 Fe2 Fe2 5_554 . 2_555 90.000(7) ?
Mn2 Fe2 Fe2 5_554 . 3_555 61.148(4) ?
Mn2 Fe2 Fe2 5_554 . 5_554 0 ?
Mn2 Fe2 Fe2 5_554 . 5_555 112.275(5) ?
Mn2 Fe2 Fe2 5_554 . 6_554 57.704(5) ?
Mn2 Fe2 Fe2 5_554 . 6_555 147.647(10) ?
Mn2 Fe2 Si1 5_554 . . 106.177(5) ?
Mn2 Fe2 Si1 5_554 . 2_545 59.608(4) ?
Mn2 Fe2 Si1 5_554 . 3_665 117.077(6) ?
Mn2 Fe2 Si1 5_554 . 4_654 51.371(6) ?
Mn2 Fe2 Si1 5_554 . 4_655 150.283(5) ?
Mn2 Fe2 Mn2 5_555 . 6_554 147.647(10) ?
Mn2 Fe2 Mn2 5_555 . 6_555 57.704(5) ?
Mn2 Fe2 Fe2 5_555 . 2_555 90.000(7) ?
Mn2 Fe2 Fe2 5_555 . 3_555 61.148(4) ?
Mn2 Fe2 Fe2 5_555 . 5_554 112.275(5) ?
Mn2 Fe2 Fe2 5_555 . 5_555 0 ?
Mn2 Fe2 Fe2 5_555 . 6_554 147.647(10) ?
Mn2 Fe2 Fe2 5_555 . 6_555 57.704(5) ?
Mn2 Fe2 Si1 5_555 . . 106.177(5) ?
Mn2 Fe2 Si1 5_555 . 2_545 59.608(4) ?
Mn2 Fe2 Si1 5_555 . 3_665 117.077(6) ?
Mn2 Fe2 Si1 5_555 . 4_654 150.283(5) ?
Mn2 Fe2 Si1 5_555 . 4_655 51.371(6) ?
Mn2 Fe2 Mn2 6_554 . 6_555 112.275(7) ?
Mn2 Fe2 Fe2 6_554 . 2_555 61.148(6) ?
Mn2 Fe2 Fe2 6_554 . 3_555 90.000(7) ?
Mn2 Fe2 Fe2 6_554 . 5_554 57.704(5) ?
Mn2 Fe2 Fe2 6_554 . 5_555 147.647(10) ?
Mn2 Fe2 Fe2 6_554 . 6_554 0 ?
Mn2 Fe2 Fe2 6_554 . 6_555 112.275(7) ?
Mn2 Fe2 Si1 6_554 . . 106.177(6) ?
Mn2 Fe2 Si1 6_554 . 2_545 117.077(5) ?
Mn2 Fe2 Si1 6_554 . 3_665 59.608(4) ?
Mn2 Fe2 Si1 6_554 . 4_654 51.371(8) ?
Mn2 Fe2 Si1 6_554 . 4_655 150.283(4) ?
Mn2 Fe2 Fe2 6_555 . 2_555 61.148(6) ?
Mn2 Fe2 Fe2 6_555 . 3_555 90.000(7) ?
Mn2 Fe2 Fe2 6_555 . 5_554 147.647(10) ?
Mn2 Fe2 Fe2 6_555 . 5_555 57.704(5) ?
Mn2 Fe2 Fe2 6_555 . 6_554 112.275(7) ?
Mn2 Fe2 Fe2 6_555 . 6_555 0 ?
Mn2 Fe2 Si1 6_555 . . 106.177(6) ?
Mn2 Fe2 Si1 6_555 . 2_545 117.077(5) ?
Mn2 Fe2 Si1 6_555 . 3_665 59.608(4) ?
Mn2 Fe2 Si1 6_555 . 4_654 150.283(4) ?
Mn2 Fe2 Si1 6_555 . 4_655 51.371(8) ?
Fe2 Fe2 Fe2 2_555 . 3_555 60.000(7) ?
Fe2 Fe2 Fe2 2_555 . 5_554 90.000(7) ?
Fe2 Fe2 Fe2 2_555 . 5_555 90.000(7) ?
Fe2 Fe2 Fe2 2_555 . 6_554 61.148(6) ?
Fe2 Fe2 Fe2 2_555 . 6_555 61.148(6) ?
Fe2 Fe2 Si1 2_555 . . 150.000(3) ?
Fe2 Fe2 Si1 2_555 . 2_545 114.777(10) ?
Fe2 Fe2 Si1 2_555 . 3_665 54.777(11) ?
Fe2 Fe2 Si1 2_555 . 4_654 112.306(7) ?
Fe2 Fe2 Si1 2_555 . 4_655 112.306(7) ?
Fe2 Fe2 Fe2 3_555 . 5_554 61.148(4) ?
Fe2 Fe2 Fe2 3_555 . 5_555 61.148(4) ?
Fe2 Fe2 Fe2 3_555 . 6_554 90.000(7) ?
Fe2 Fe2 Fe2 3_555 . 6_555 90.000(7) ?
Fe2 Fe2 Si1 3_555 . . 150.000(6) ?
Fe2 Fe2 Si1 3_555 . 2_545 54.777(8) ?
Fe2 Fe2 Si1 3_555 . 3_665 114.777(13) ?
Fe2 Fe2 Si1 3_555 . 4_654 112.306(7) ?
Fe2 Fe2 Si1 3_555 . 4_655 112.306(7) ?
Fe2 Fe2 Fe2 5_554 . 5_555 112.275(5) ?
Fe2 Fe2 Fe2 5_554 . 6_554 57.704(5) ?
Fe2 Fe2 Fe2 5_554 . 6_555 147.647(10) ?
Fe2 Fe2 Si1 5_554 . . 106.177(5) ?
Fe2 Fe2 Si1 5_554 . 2_545 59.608(4) ?
Fe2 Fe2 Si1 5_554 . 3_665 117.077(6) ?
Fe2 Fe2 Si1 5_554 . 4_654 51.371(6) ?
Fe2 Fe2 Si1 5_554 . 4_655 150.283(5) ?
Fe2 Fe2 Fe2 5_555 . 6_554 147.647(10) ?
Fe2 Fe2 Fe2 5_555 . 6_555 57.704(5) ?
Fe2 Fe2 Si1 5_555 . . 106.177(5) ?
Fe2 Fe2 Si1 5_555 . 2_545 59.608(4) ?
Fe2 Fe2 Si1 5_555 . 3_665 117.077(6) ?
Fe2 Fe2 Si1 5_555 . 4_654 150.283(5) ?
Fe2 Fe2 Si1 5_555 . 4_655 51.371(6) ?
Fe2 Fe2 Fe2 6_554 . 6_555 112.275(7) ?
Fe2 Fe2 Si1 6_554 . . 106.177(6) ?
Fe2 Fe2 Si1 6_554 . 2_545 117.077(5) ?
Fe2 Fe2 Si1 6_554 . 3_665 59.608(4) ?
Fe2 Fe2 Si1 6_554 . 4_654 51.371(8) ?
Fe2 Fe2 Si1 6_554 . 4_655 150.283(4) ?
Fe2 Fe2 Si1 6_555 . . 106.177(6) ?
Fe2 Fe2 Si1 6_555 . 2_545 117.077(5) ?
Fe2 Fe2 Si1 6_555 . 3_665 59.608(4) ?
Fe2 Fe2 Si1 6_555 . 4_654 150.283(4) ?
Fe2 Fe2 Si1 6_555 . 4_655 51.371(8) ?
Si1 Fe2 Si1 . . 2_545 95.223(8) ?
Si1 Fe2 Si1 . . 3_665 95.223(11) ?
Si1 Fe2 Si1 . . 4_654 64.006(9) ?
Si1 Fe2 Si1 . . 4_655 64.006(9) ?
Si1 Fe2 Si1 2_545 . 3_665 169.555(15) ?
Si1 Fe2 Si1 2_545 . 4_654 92.286(3) ?
Si1 Fe2 Si1 2_545 . 4_655 92.286(3) ?
Si1 Fe2 Si1 3_665 . 4_654 92.286(5) ?
Si1 Fe2 Si1 3_665 . 4_655 92.286(5) ?
Si1 Fe2 Si1 4_654 . 4_655 128.013(14) ?
Fe1 Si1 Fe1 . . 4_655 147.547(18) ?
Fe1 Si1 Fe1 . . 13_655 110.771(8) ?
Fe1 Si1 Fe1 . . 16_555 59.283(3) ?
Fe1 Si1 Mn1 . . . 0 ?
Fe1 Si1 Mn1 . . 4_655 147.547(18) ?
Fe1 Si1 Mn1 . . 13_655 110.771(8) ?
Fe1 Si1 Mn1 . . 16_555 59.283(3) ?
Fe1 Si1 Mn2 . . . 73.774(9) ?
Fe1 Si1 Mn2 . . 2_655 75.736(6) ?
Fe1 Si1 Mn2 . . 3_655 134.663(12) ?
Fe1 Si1 Mn2 . . 4_654 71.212(3) ?
Fe1 Si1 Mn2 . . 4_655 124.542(3) ?
Fe1 Si1 Fe2 . . . 73.774(9) ?
Fe1 Si1 Fe2 . . 2_655 75.736(6) ?
Fe1 Si1 Fe2 . . 3_655 134.663(12) ?
Fe1 Si1 Fe2 . . 4_654 71.212(3) ?
Fe1 Si1 Fe2 . . 4_655 124.542(3) ?
Fe1 Si1 Si1 . . 4_654 55.386(4) ?
Fe1 Si1 Si1 . . 4_655 107.046(10) ?
Fe1 Si1 Fe1 4_655 . 13_655 59.283(3) ?
Fe1 Si1 Fe1 4_655 . 16_555 110.771(8) ?
Fe1 Si1 Mn1 4_655 . . 147.547(18) ?
Fe1 Si1 Mn1 4_655 . 4_655 0 ?
Fe1 Si1 Mn1 4_655 . 13_655 59.283(3) ?
Fe1 Si1 Mn1 4_655 . 16_555 110.771(8) ?
Fe1 Si1 Mn2 4_655 . . 73.773(9) ?
Fe1 Si1 Mn2 4_655 . 2_655 134.663(12) ?
Fe1 Si1 Mn2 4_655 . 3_655 75.736(5) ?
Fe1 Si1 Mn2 4_655 . 4_654 124.542(3) ?
Fe1 Si1 Mn2 4_655 . 4_655 71.212(3) ?
Fe1 Si1 Fe2 4_655 . . 73.773(9) ?
Fe1 Si1 Fe2 4_655 . 2_655 134.663(12) ?
Fe1 Si1 Fe2 4_655 . 3_655 75.736(5) ?
Fe1 Si1 Fe2 4_655 . 4_654 124.542(3) ?
Fe1 Si1 Fe2 4_655 . 4_655 71.212(3) ?
Fe1 Si1 Si1 4_655 . 4_654 107.046(10) ?
Fe1 Si1 Si1 4_655 . 4_655 55.386(4) ?
Fe1 Si1 Fe1 13_655 . 16_555 147.547(18) ?
Fe1 Si1 Mn1 13_655 . . 110.771(8) ?
Fe1 Si1 Mn1 13_655 . 4_655 59.283(3) ?
Fe1 Si1 Mn1 13_655 . 13_655 0 ?
Fe1 Si1 Mn1 13_655 . 16_555 147.547(18) ?
Fe1 Si1 Mn2 13_655 . . 73.773(9) ?
Fe1 Si1 Mn2 13_655 . 2_655 134.663(12) ?
Fe1 Si1 Mn2 13_655 . 3_655 75.736(5) ?
Fe1 Si1 Mn2 13_655 . 4_654 71.212(3) ?
Fe1 Si1 Mn2 13_655 . 4_655 124.542(3) ?
Fe1 Si1 Fe2 13_655 . . 73.773(9) ?
Fe1 Si1 Fe2 13_655 . 2_655 134.663(12) ?
Fe1 Si1 Fe2 13_655 . 3_655 75.736(5) ?
Fe1 Si1 Fe2 13_655 . 4_654 71.212(3) ?
Fe1 Si1 Fe2 13_655 . 4_655 124.542(3) ?
Fe1 Si1 Si1 13_655 . 4_654 55.386(4) ?
Fe1 Si1 Si1 13_655 . 4_655 107.046(10) ?
Fe1 Si1 Mn1 16_555 . . 59.283(3) ?
Fe1 Si1 Mn1 16_555 . 4_655 110.771(8) ?
Fe1 Si1 Mn1 16_555 . 13_655 147.547(18) ?
Fe1 Si1 Mn1 16_555 . 16_555 0 ?
Fe1 Si1 Mn2 16_555 . . 73.774(9) ?
Fe1 Si1 Mn2 16_555 . 2_655 75.736(6) ?
Fe1 Si1 Mn2 16_555 . 3_655 134.663(12) ?
Fe1 Si1 Mn2 16_555 . 4_654 124.542(3) ?
Fe1 Si1 Mn2 16_555 . 4_655 71.212(3) ?
Fe1 Si1 Fe2 16_555 . . 73.774(9) ?
Fe1 Si1 Fe2 16_555 . 2_655 75.736(6) ?
Fe1 Si1 Fe2 16_555 . 3_655 134.663(12) ?
Fe1 Si1 Fe2 16_555 . 4_654 124.542(3) ?
Fe1 Si1 Fe2 16_555 . 4_655 71.212(3) ?
Fe1 Si1 Si1 16_555 . 4_654 107.046(10) ?
Fe1 Si1 Si1 16_555 . 4_655 55.386(4) ?
Mn1 Si1 Mn1 . . 4_655 147.547(18) ?
Mn1 Si1 Mn1 . . 13_655 110.771(8) ?
Mn1 Si1 Mn1 . . 16_555 59.283(3) ?
Mn1 Si1 Mn2 . . . 73.774(9) ?
Mn1 Si1 Mn2 . . 2_655 75.736(6) ?
Mn1 Si1 Mn2 . . 3_655 134.663(12) ?
Mn1 Si1 Mn2 . . 4_654 71.212(3) ?
Mn1 Si1 Mn2 . . 4_655 124.542(3) ?
Mn1 Si1 Fe2 . . . 73.774(9) ?
Mn1 Si1 Fe2 . . 2_655 75.736(6) ?
Mn1 Si1 Fe2 . . 3_655 134.663(12) ?
Mn1 Si1 Fe2 . . 4_654 71.212(3) ?
Mn1 Si1 Fe2 . . 4_655 124.542(3) ?
Mn1 Si1 Si1 . . 4_654 55.386(4) ?
Mn1 Si1 Si1 . . 4_655 107.046(10) ?
Mn1 Si1 Mn1 4_655 . 13_655 59.283(3) ?
Mn1 Si1 Mn1 4_655 . 16_555 110.771(8) ?
Mn1 Si1 Mn2 4_655 . . 73.773(9) ?
Mn1 Si1 Mn2 4_655 . 2_655 134.663(12) ?
Mn1 Si1 Mn2 4_655 . 3_655 75.736(5) ?
Mn1 Si1 Mn2 4_655 . 4_654 124.542(3) ?
Mn1 Si1 Mn2 4_655 . 4_655 71.212(3) ?
Mn1 Si1 Fe2 4_655 . . 73.773(9) ?
Mn1 Si1 Fe2 4_655 . 2_655 134.663(12) ?
Mn1 Si1 Fe2 4_655 . 3_655 75.736(5) ?
Mn1 Si1 Fe2 4_655 . 4_654 124.542(3) ?
Mn1 Si1 Fe2 4_655 . 4_655 71.212(3) ?
Mn1 Si1 Si1 4_655 . 4_654 107.046(10) ?
Mn1 Si1 Si1 4_655 . 4_655 55.386(4) ?
Mn1 Si1 Mn1 13_655 . 16_555 147.547(18) ?
Mn1 Si1 Mn2 13_655 . . 73.773(9) ?
Mn1 Si1 Mn2 13_655 . 2_655 134.663(12) ?
Mn1 Si1 Mn2 13_655 . 3_655 75.736(5) ?
Mn1 Si1 Mn2 13_655 . 4_654 71.212(3) ?
Mn1 Si1 Mn2 13_655 . 4_655 124.542(3) ?
Mn1 Si1 Fe2 13_655 . . 73.773(9) ?
Mn1 Si1 Fe2 13_655 . 2_655 134.663(12) ?
Mn1 Si1 Fe2 13_655 . 3_655 75.736(5) ?
Mn1 Si1 Fe2 13_655 . 4_654 71.212(3) ?
Mn1 Si1 Fe2 13_655 . 4_655 124.542(3) ?
Mn1 Si1 Si1 13_655 . 4_654 55.386(4) ?
Mn1 Si1 Si1 13_655 . 4_655 107.046(10) ?
Mn1 Si1 Mn2 16_555 . . 73.774(9) ?
Mn1 Si1 Mn2 16_555 . 2_655 75.736(6) ?
Mn1 Si1 Mn2 16_555 . 3_655 134.663(12) ?
Mn1 Si1 Mn2 16_555 . 4_654 124.542(3) ?
Mn1 Si1 Mn2 16_555 . 4_655 71.212(3) ?
Mn1 Si1 Fe2 16_555 . . 73.774(9) ?
Mn1 Si1 Fe2 16_555 . 2_655 75.736(6) ?
Mn1 Si1 Fe2 16_555 . 3_655 134.663(12) ?
Mn1 Si1 Fe2 16_555 . 4_654 124.542(3) ?
Mn1 Si1 Fe2 16_555 . 4_655 71.212(3) ?
Mn1 Si1 Si1 16_555 . 4_654 107.046(10) ?
Mn1 Si1 Si1 16_555 . 4_655 55.386(4) ?
Mn2 Si1 Mn2 . . 2_655 144.777(7) ?
Mn2 Si1 Mn2 . . 3_655 144.777(7) ?
Mn2 Si1 Mn2 . . 4_654 115.994(9) ?
Mn2 Si1 Mn2 . . 4_655 115.994(9) ?
Mn2 Si1 Fe2 . . . 0 ?
Mn2 Si1 Fe2 . . 2_655 144.777(7) ?
Mn2 Si1 Fe2 . . 3_655 144.777(7) ?
Mn2 Si1 Fe2 . . 4_654 115.994(9) ?
Mn2 Si1 Fe2 . . 4_655 115.994(9) ?
Mn2 Si1 Si1 . . 4_654 60.533(10) ?
Mn2 Si1 Si1 . . 4_655 60.533(10) ?
Mn2 Si1 Mn2 2_655 . 3_655 70.445(12) ?
Mn2 Si1 Mn2 2_655 . 4_654 69.021(8) ?
Mn2 Si1 Mn2 2_655 . 4_655 69.021(8) ?
Mn2 Si1 Fe2 2_655 . . 144.777(7) ?
Mn2 Si1 Fe2 2_655 . 2_655 0 ?
Mn2 Si1 Fe2 2_655 . 3_655 70.445(12) ?
Mn2 Si1 Fe2 2_655 . 4_654 69.021(8) ?
Mn2 Si1 Fe2 2_655 . 4_655 69.021(8) ?
Mn2 Si1 Si1 2_655 . 4_654 113.694(7) ?
Mn2 Si1 Si1 2_655 . 4_655 113.694(7) ?
Mn2 Si1 Mn2 3_655 . 4_654 69.021(8) ?
Mn2 Si1 Mn2 3_655 . 4_655 69.021(8) ?
Mn2 Si1 Fe2 3_655 . . 144.777(7) ?
Mn2 Si1 Fe2 3_655 . 2_655 70.445(12) ?
Mn2 Si1 Fe2 3_655 . 3_655 0 ?
Mn2 Si1 Fe2 3_655 . 4_654 69.021(8) ?
Mn2 Si1 Fe2 3_655 . 4_655 69.021(8) ?
Mn2 Si1 Si1 3_655 . 4_654 113.694(7) ?
Mn2 Si1 Si1 3_655 . 4_655 113.694(7) ?
Mn2 Si1 Mn2 4_654 . 4_655 128.013(16) ?
Mn2 Si1 Fe2 4_654 . . 115.994(9) ?
Mn2 Si1 Fe2 4_654 . 2_655 69.021(8) ?
Mn2 Si1 Fe2 4_654 . 3_655 69.021(8) ?
Mn2 Si1 Fe2 4_654 . 4_654 0 ?
Mn2 Si1 Fe2 4_654 . 4_655 128.013(16) ?
Mn2 Si1 Si1 4_654 . 4_654 55.460(8) ?
Mn2 Si1 Si1 4_654 . 4_655 176.527(17) ?
Mn2 Si1 Fe2 4_655 . . 115.994(9) ?
Mn2 Si1 Fe2 4_655 . 2_655 69.021(8) ?
Mn2 Si1 Fe2 4_655 . 3_655 69.021(8) ?
Mn2 Si1 Fe2 4_655 . 4_654 128.013(16) ?
Mn2 Si1 Fe2 4_655 . 4_655 0 ?
Mn2 Si1 Si1 4_655 . 4_654 176.527(17) ?
Mn2 Si1 Si1 4_655 . 4_655 55.460(8) ?
Fe2 Si1 Fe2 . . 2_655 144.777(7) ?
Fe2 Si1 Fe2 . . 3_655 144.777(7) ?
Fe2 Si1 Fe2 . . 4_654 115.994(9) ?
Fe2 Si1 Fe2 . . 4_655 115.994(9) ?
Fe2 Si1 Si1 . . 4_654 60.533(10) ?
Fe2 Si1 Si1 . . 4_655 60.533(10) ?
Fe2 Si1 Fe2 2_655 . 3_655 70.445(12) ?
Fe2 Si1 Fe2 2_655 . 4_654 69.021(8) ?
Fe2 Si1 Fe2 2_655 . 4_655 69.021(8) ?
Fe2 Si1 Si1 2_655 . 4_654 113.694(7) ?
Fe2 Si1 Si1 2_655 . 4_655 113.694(7) ?
Fe2 Si1 Fe2 3_655 . 4_654 69.021(8) ?
Fe2 Si1 Fe2 3_655 . 4_655 69.021(8) ?
Fe2 Si1 Si1 3_655 . 4_654 113.694(7) ?
Fe2 Si1 Si1 3_655 . 4_655 113.694(7) ?
Fe2 Si1 Fe2 4_654 . 4_655 128.013(16) ?
Fe2 Si1 Si1 4_654 . 4_654 55.460(8) ?
Fe2 Si1 Si1 4_654 . 4_655 176.527(17) ?
Fe2 Si1 Si1 4_655 . 4_654 176.527(17) ?
Fe2 Si1 Si1 4_655 . 4_655 55.460(8) ?
Si1 Si1 Si1 4_654 . 4_655 121.067(17) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Fe1 Fe1 . 16_554 2.37780(10) ?
Fe1 Fe1 . 16_555 2.37780(10) ?
Fe1 Mn1 . . 0 ?
Fe1 Mn1 . 16_554 2.37780(10) ?
Fe1 Mn1 . 16_555 2.37780(10) ?
Fe1 Mn2 . . 2.94629(17) ?
Fe1 Mn2 . 2_655 2.94629(15) ?
Fe1 Mn2 . 3_665 2.9463(2) ?
Fe1 Mn2 . 4_654 2.94629(15) ?
Fe1 Mn2 . 5_664 2.94629(17) ?
Fe1 Mn2 . 6_554 2.9463(2) ?
Fe1 Fe2 . . 2.94629(17) ?
Fe1 Fe2 . 2_655 2.94629(15) ?
Fe1 Fe2 . 3_665 2.9463(2) ?
Fe1 Fe2 . 4_654 2.94629(15) ?
Fe1 Fe2 . 5_664 2.94629(17) ?
Fe1 Fe2 . 6_554 2.9463(2) ?
Fe1 Si1 . . 2.40391(13) ?
Fe1 Si1 . 2_655 2.40391(14) ?
Fe1 Si1 . 3_665 2.4039(4) ?
Fe1 Si1 . 4_654 2.40391(14) ?
Fe1 Si1 . 5_664 2.40391(13) ?
Fe1 Si1 . 6_554 2.4039(4) ?
Mn2 Mn1 . . 2.94629(17) ?
Mn2 Mn1 . 4_655 2.94629(15) ?
Mn2 Mn1 . 13_655 2.94629(15) ?
Mn2 Mn1 . 16_555 2.94629(17) ?
Mn2 Mn2 . 2_555 2.7636(3) ?
Mn2 Mn2 . 3_555 2.7636(3) ?
Mn2 Mn2 . 5_554 2.86352(13) ?
Mn2 Mn2 . 5_555 2.86352(13) ?
Mn2 Mn2 . 6_554 2.86352(17) ?
Mn2 Mn2 . 6_555 2.86352(17) ?
Mn2 Fe2 . . 0 ?
Mn2 Fe2 . 2_555 2.7636(3) ?
Mn2 Fe2 . 3_555 2.7636(3) ?
Mn2 Fe2 . 5_554 2.86352(13) ?
Mn2 Fe2 . 5_555 2.86352(13) ?
Mn2 Fe2 . 6_554 2.86352(17) ?
Mn2 Fe2 . 6_555 2.86352(17) ?
Mn2 Si1 . . 2.5029(4) ?
Mn2 Si1 . 2_545 2.3958(3) ?
Mn2 Si1 . 3_665 2.3958(4) ?
Mn2 Si1 . 4_654 2.6454(2) ?
Mn2 Si1 . 4_655 2.6454(2) ?
Si1 Mn1 . . 2.40391(13) ?
Si1 Mn1 . 4_655 2.40391(14) ?
Si1 Mn1 . 13_655 2.40391(14) ?
Si1 Mn1 . 16_555 2.40391(13) ?
Si1 Fe2 . . 2.5029(4) ?
Si1 Fe2 . 2_655 2.3958(3) ?
Si1 Fe2 . 3_655 2.3958(4) ?
Si1 Fe2 . 4_654 2.6454(2) ?
Si1 Fe2 . 4_655 2.6454(2) ?
Si1 Si1 . 4_654 2.7311(3) ?
Si1 Si1 . 4_655 2.7311(3) ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?
loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_c_label
_jana_atom_site_adp_c_type_symbol
_jana_atom_site_adp_c_111
_jana_atom_site_adp_c_112
_jana_atom_site_adp_c_113
_jana_atom_site_adp_c_122
_jana_atom_site_adp_c_123
_jana_atom_site_adp_c_133
_jana_atom_site_adp_c_222
_jana_atom_site_adp_c_223
_jana_atom_site_adp_c_233
_jana_atom_site_adp_c_333
? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_d_label
_jana_atom_site_adp_d_type_symbol
_jana_atom_site_adp_d_1111
_jana_atom_site_adp_d_1112
_jana_atom_site_adp_d_1113
_jana_atom_site_adp_d_1122
_jana_atom_site_adp_d_1123
_jana_atom_site_adp_d_1133
_jana_atom_site_adp_d_1222
_jana_atom_site_adp_d_1223
_jana_atom_site_adp_d_1233
_jana_atom_site_adp_d_1333
_jana_atom_site_adp_d_2222
_jana_atom_site_adp_d_2223
_jana_atom_site_adp_d_2233
_jana_atom_site_adp_d_2333
_jana_atom_site_adp_d_3333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_e_label
_jana_atom_site_adp_e_type_symbol
_jana_atom_site_adp_e_11111
_jana_atom_site_adp_e_11112
_jana_atom_site_adp_e_11113
_jana_atom_site_adp_e_11122
_jana_atom_site_adp_e_11123
_jana_atom_site_adp_e_11133
_jana_atom_site_adp_e_11222
_jana_atom_site_adp_e_11223
_jana_atom_site_adp_e_11233
_jana_atom_site_adp_e_11333
_jana_atom_site_adp_e_12222
_jana_atom_site_adp_e_12223
_jana_atom_site_adp_e_12233
_jana_atom_site_adp_e_12333
_jana_atom_site_adp_e_13333
_jana_atom_site_adp_e_22222
_jana_atom_site_adp_e_22223
_jana_atom_site_adp_e_22233
_jana_atom_site_adp_e_22333
_jana_atom_site_adp_e_23333
_jana_atom_site_adp_e_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_f_label
_jana_atom_site_adp_f_type_symbol
_jana_atom_site_adp_f_111111
_jana_atom_site_adp_f_111112
_jana_atom_site_adp_f_111113
_jana_atom_site_adp_f_111122
_jana_atom_site_adp_f_111123
_jana_atom_site_adp_f_111133
_jana_atom_site_adp_f_111222
_jana_atom_site_adp_f_111223
_jana_atom_site_adp_f_111233
_jana_atom_site_adp_f_111333
_jana_atom_site_adp_f_112222
_jana_atom_site_adp_f_112223
_jana_atom_site_adp_f_112233
_jana_atom_site_adp_f_112333
_jana_atom_site_adp_f_113333
_jana_atom_site_adp_f_122222
_jana_atom_site_adp_f_122223
_jana_atom_site_adp_f_122233
_jana_atom_site_adp_f_122333
_jana_atom_site_adp_f_123333
_jana_atom_site_adp_f_133333
_jana_atom_site_adp_f_222222
_jana_atom_site_adp_f_222223
_jana_atom_site_adp_f_222233
_jana_atom_site_adp_f_222333
_jana_atom_site_adp_f_223333
_jana_atom_site_adp_f_233333
_jana_atom_site_adp_f_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

_cod_database_fobs_code 2300726
